Abstract
In secondorder quantum phase transitions from magnetically ordered to paramagnetic states at T = 0, tuned by pressure or chemical substitution, a quantum critical point is expected to appear with critical behavior manifesting in the slowing down of spin fluctuations in the paramagnetic state and a continuous development of the order parameter in the ordered state. Quantum criticality is discussed widely as a possible driving force for unconventional superconductivity and other exotic phenomena in correlated electron systems. In the real world, however, quantum critical points and quantum criticality are often masked by a preceding firstorder transition and/or the development of competing states. Pressure tuning of the itinerantelectron helical magnet MnSi is a wellknown example of the suppression of a quantum critical point due to a firstorder phase transition and resulting destruction of the ordered state. Utilizing muon spin relaxation experiments, here we report that 15% Fesubstituted (Mn,Fe)Si exhibits completely different behavior with pressure tuning, including the restoration of secondorder quantum critical behavior and a quantum critical point at p _{ QPC } ~ 21–23 kbar, which coincides with the T = 0 crossing point of the extrapolated phase boundary line of pure MnSi. This result is quantitatively consistent with the recent theory of itinerantelectron ferromagnets by Sang, Belitz, and Kirkpatrick, who argued that disorder would restore a quantum critical point which is otherwise hidden by a firstorder transition.
Introduction
A firstorder phase transition is associated with a discontinuous change of the order parameter (such as staggered magnetization), while a secondorder transition involves the slowing down of critical fluctuations at the phase boundary and a continuous development of the order parameter from zero in the disordered phase to nonzero values in the ordered phase. Whereas thermal phase transitions are achieved by changing the temperature T, quantum phase transitions occur when the phase boundary is crossed at T → 0 by tuning nonthermal parameters, such as pressure or chemical composition. Quantum phase transitions have become an important topic in modern condensed matter physics. In addition to unconventional superconductors,^{1,2,3} heavyfermion systems,^{4, 5} and Mott transition systems,^{6} extensive studies of thermal and quantum phase transitions have been conducted on itinerantelectron magnets, theoretically by Moriya^{7} and Belitz, Kirkpatrick and others,^{8, 9} and experimentally in MnSi tuned by temperature^{10} and pressure^{11,12,13} and in (Mn,Fe)Si,^{14} (Sr,Ca)RuO_{3} ^{13} and (Sc,Lu)_{3}In^{15} by chemical substitution and/or pressure.
MnSi is a representative metallic magnet which has a small ordered moment (~0.4 Bohr magneton per formula unit at T = 0) and a helical spin structure below a relatively low ordering temperature T _{ C } ~ 29 K in ambient pressure. From 1970–1990, the thermal transition in this system was studied by neutron scattering^{16} and muon spin relaxation (MuSR),^{17} which observed secondorderlike critical behavior and paramagnetic spin fluctuations, consistent with predictions of the selfconsistent renormalization theory^{7} developed for metallic ferromagnets. In 1997, Pfleiderer et al.^{11} discovered that the magnetic order of MnSi can be suppressed by the application of hydrostatic pressure beyond a critical pressure p _{ c } ~ 15 kbar, as shown in the phase diagram of Fig. 1a. MnSi has a hierarchy of energy scales, starting from the strongest ferromagnetic exchange interaction J, followed by the Dzyaloshinskii–Moriya interaction D which leads to helical spin correlations, and finally the crystal anisotropy I, which stabilizes the moment direction. The interplay of these energy scales, combined with the B20 crystal structure that lacks inversion symmetry, results in a variety of novel phenomena, including a Skyrmion lattice state in applied magnetic fields below T _{ C } ^{18, 19} and chiral spin fluctuations/Skyrmion liquid above T _{ C }.^{20,21,22}
At temperatures 1–2 K above T _{ C } in ambient pressure, the spin correlation length ξ in MnSi becomes comparable to the pitch length l ~ 18 nm of the helical spiral, transforming the ferromagnetic critical behavior into helical spin fluctuations. The process of stabilizing the helical fluctuations by I leads to weakly firstorder behavior at T _{ C }, as detected by neutron scattering (chiral fluctuations),^{10, 20,21,22} transport (sharp peaking in the Tderivative of the resistivity),^{11, 23} and specific heat^{23} (a shoulder above T _{ C } with a sharp peak at T _{ C }). In MuSR studies, this feature is manifest as a discontinuous change of the order parameter below T _{ C } ^{24} and a modification of the critical exponent above T _{ C }.^{25, 26} The spin correlation time τ, however, keeps increasing with decreasing T even in this narrow temperature region above T _{ C },^{22} resulting in a peak of the muon spin relaxation rate 1/T _{ 1 } at T _{ C }.^{13, 17, 25, 26} This narrow temperature region above T _{ C } is illustrated by the pink region (HF) in Fig. 1a.
As the pressure is increased above p*, the ac susceptibility of a clean specimen (with residual resistivity ratio RRR = 243) was observed to exhibit a clearly discontinuous change at T _{ C },^{11} indicating a firstorder thermal transition. The ordering temperature, which decreases nearly linearly with p from ambient pressure up to p*, acquires a steeper slope at p* < p < p _{ c },^{11} while neutron scattering^{12} observes a diffuse signal (initially called ‘partial order’) below the extrapolated T _{ C } (p) line (broken line in Fig. 1a). MuSR measurements with pressure^{13} showed that the “partial order”, seen in the blue region “D” in Fig. 1a, is a manifestation of slow dynamic spin fluctuations with the time scale τ ~ 10^{−10}–10^{−11} s.
Zerofield nuclear magnetic resonance (NMR)^{27} and MuSR^{13, 28} measurements in MnSi found that the magnitude of the static internal magnetic field at T → 0, which is proportional to the ordered moment size, exhibits only a slight reduction with increasing p at p* < p < p _{ c }, followed by an abrupt reduction to zero above p _{ c }. This discontinuous change of the order parameter at p _{ c } clearly demonstrates the firstorder character of the quantum phase transition in MnSi tuned with pressure p. Signatures of phase separation between ordered and disordered volumes were reported from MuSR^{13} and NMR^{27} experiments at p* < p < p _{ c }, corresponding to the green region “P” in Fig. 1a. Neutron scattering observed a continuous variation of the helical Bragg peak intensity I _{ B } at T = 2 K near p _{ c }.^{29, 30} This, however, cannot be taken as evidence for a secondorder quantum transition, since I _{ B } ∝ S ^{2} × V _{ ord } is proportional to the product of the square of the ordered moment S and the volume fraction V _{ ord } of the ordered region, and neutron studies cannot distinguish between contributions from S and V _{ ord }. In the case of MnSi, the continuous variation of I _{ B } is due to the discontinuous change of S at p _{ c } multiplied by the continuous development of V _{ ord } below p = p _{ c }.
Results
In this paper, we report MuSR measurements of (Mn,Fe)Si with 15% Fe in ambient and hydrostatic pressure. We find that this Fedoped sample exhibits drastically different behavior than the abovementioned results in pure MnSi. Although both (Mn,Fe) substitution^{14} and the application of pressure suppress the magnetic order in MnSi, these two tuning methods could be different, as the former varies both the carrier density and lattice constant,^{31} while the latter mainly alters the band width, in a way reminiscent of filling and bandwidth control in Mott transitions.^{6} As shown in Fig. 1a, iron substitution suppresses T _{ C } in (Mn_{0.85}Fe_{0.15})Si to T _{C} ~ 4 K at ambient pressure. At the genral purpose decaychannel (GPD) instrument of the Paul Scherrer Institut (PSI), we carried out MuSR measurements in zero field (ZF) and longitudinal field (LF) on a single crystal specimen of (Mn_{0.85}Fe_{0.15})Si in hydrostatic pressure p using a standard piston pressure cell and a ^{3}He cryostat.^{32} Details of the MuSR method, crystal preparation, and the pressure cell are described in the “Methods” section. The static magnetic order in (Mn_{0.85}Fe_{0.15})Si survives up to p _{ c } = 21–23 kbar with clear signatures of dynamic critical behavior, a continuous evolution of the ordered moment size, and a full magnetically ordered volume fraction. These behaviors demonstrate the restoration of secondorder thermal and quantum phase transitions due presumably to substantial disorder caused by the (Mn,Fe) substitution.
Figure 2a–e displays representative zerofield (ZF) MuSR time spectra from (Mn,Fe)Si in ambient and applied pressure. These spectra include contributions not only from the sample but also from the pressure cell, which corresponds to about 45% of the total signal amplitude. The ZF MuSR spectra under ambient pressure (Fig. 2a) show fast relaxation below T _{ C } ~ 4 K and a strongly overdamped oscillation at 0.25 K. This indicates that the static internal magnetic field of (Mn_{0.85}Fe_{0.15})Si has a broad distribution, in contrast to that of MnSi, which may be attributed to spatially random (Mn,Fe) substitutions. The spectra at p = 11.7 kbar in Fig. 2b, in the vicinity of p* for pure MnSi, are qualitatively the same as at ambient pressure, but without any clear oscillation observed down to T = 0.25 K. As shown in Fig. 2c, d, fast relaxation is observed in (Mn,Fe)Si even at p = 16.4 and 19.3 kbar, i.e., pressures higher than the critical pressure p _{ c } for pure MnSi. The fast relaxation in ZF at low temperature finally disappears at p = 23 kbar (Fig. 2e). The ZF relaxation at T = 0.25 K for p = 0–19.3 kbar can be substantially restored (decoupled) by the application of a small LF = 500 G, as shown in Fig. 2f, which confirms that static magnetic order is the origin of the observed ZF relaxation at low temperatures. The absence of fast relaxation in ZF at p = 23 kbar also confirms that muons landing in the pressure cell do not make significant contributions to the observed temperature dependence of the MuSR spectra.
We analyzed the ZFMuSR spectra P(t) with the formula
where A _{ sp }, A _{ cl }, and A _{ bg } correspond to the initial asymmetries for the signals from the sample, pressure cell, and pressureindependent background, respectively. These parameters are fixed for all temperatures, and fixed for pressures in a given pressure cell (we used two cells), with typical contributions close to 45, 45, and 10% each of the total asymmetry signal. The time evolution of the signal from the sample, G _{ sp }(t) was fitted with the form
with f _{ mag } representing the volume fraction of the magnetically ordered region, and 1/T _{ 1 } the dynamic muon spin relaxation rate. Among a few possible choices of functional forms for representing the effect of static internal fields from the ordered moments, the best fit to the observed data were obtained by the generalized Kubo–Toyabe function G _{ gkt }(t)^{33}
where σ denotes the static relaxation rate proportional to the ordered moment size, and β is the stretching power, ranging between 1.1–1.4, which was fixed independent of temperature for a given pressure. More details of the data analysis in ZF, including estimates of the cell and background contributions, are presented in the Supplementary Information (SI) together with the fitted results of each parameter for all the pressure and temperature values.
Figure 3a shows the temperature dependence of the magnetic volume fraction V _{M} = f _{ mag } in (Mn,Fe)Si. Although the thermal transition exhibits a small spread/rounding indicated by a gradual increase of V _{M}, magnetic order occupies the full volume at T = 0.25 K for p = 0–19.3 kbar, and the system becomes fully paramagnetic at p = 23 kbar. Figure 3b shows that the width σ of the static internal field, proportional to the order parameter, exhibits a nearly linear increase with decreasing temperature below T _{ C }. The values of V _{M} and σ at T = 0.25 K are shown in Fig. 3c as a function of pressure p. These results include clear signatures of secondorder quantum critical behavior: an abrupt reduction of V _{M} from 1.0 to zero across p ~ 20 kbar, and a continuous increase of σ (T → 0) from 0 to nonzero values as p is decreased below the critical pressure. The pressuretuned destruction of the magnetic order with a continuous reduction of the order parameter σ in (Mn,Fe)Si, shown in Fig. 3c, is in clear contrast to the “volumewise destruction” of magnetic order in pure MnSi, shown in Fig. 3e. The former is expected for second order quantum criticality, and the latter for firstorder quantum evolution.
To study the effects of dynamic spin fluctuations in (Mn,Fe)Si, we also performed MuSR measurements in LF = 500 G, and analyzed the data with
using the fit time range of 0.1–2 μs, as illustrated in Fig. 2f for low temperatures. For the data analysis in LF, the parameter A _{ sp } was allowed to vary as a temperaturedependent parameter representing different degrees of LF decoupling for different magnitudes σ of the static internal field below T _{ C }. As shown in Fig. 3d, 1/T _{ 1 } exhibits a clear maximum due to critical slowing down of spin fluctuations around T _{ C } for all the pressure values between p = 0–19.3 kbar. Qualitatively similar behavior can also be seen in the variation of 1/T _{ 1 } in ZF shown in the SI, and the magnitude of 1/T _{ 1 } exhibits a dependence on LF similar to the known results for pure MnSi at ambient pressure.^{26} The prominent peaks in the plot of 1/T _{ 1 } vs T for (Mn,Fe)Si over a wide pressure range in Fig. 3d is in a clear contrast to the pressure dependence of 1/T _{ 1 } observed in pure MnSi^{13} replotted here in Fig. 3f, where the peaking of the relaxation rate was suppressed with increasing pressure and completely eliminated at p ~ p*. The peaking of 1/T _{ 1 } is an additional signature of the restoration of secondorder thermal critical behavior in (Mn_{0.85}Fe_{0.15})Si.
Discussion
The results for pure MnSi and the more disordered (Mn_{0.85}Fe_{0.15})Si are consistent with the theories of Belitz, Kirkpatrick and coworkers.^{8, 9, 34,35,36,37} Considering the effect of a negative m ^{3} ln(m) term of the magnetization m (order parameter) on the free energy in itinerant ferromagnets due to soft modes and particlehole excitations, they proposed that the secondorder thermal transition in ferromagnets is replaced by a firstorder transition at a tricritical point (TCP) when approaching the quantum critical point (QCP), as illustrated in Fig. 1b.^{8, 9} This behavior matches the results in pure MnSi, except for the effect of helical spin correlations, which adds a weakly firstorder character to the thermal transition before the TCP is reached, and phase separation at p* < p, which cannot be expected for ideally thermodynamic behavior in systems without disorder.^{36, 37} In their recent studies,^{36, 37} quenched disorder was suggested as a possible origin for the phase separation observed in pure MnSi. This situation is illustrated in Fig. 1b, c. Furthermore, they also recently predicted^{34, 35} that the effect of disorder weakens the negative m ^{3} ln(m) term, leading to a reduction of the region between the TCP and QCP, and finally leads to a disappearance of the TCP as illustrated in Fig 1d. The present results showing the restoration of secondorder quantum criticality in (Mn_{0.85}Fe_{0.15})Si are qualitatively consistent with this prediction.
The residual resistivity of the present singlecrystal specimen of (Mn_{0.85}Fe_{0.15})Si is estimated to be 60–100 μΩ cm, from the published results^{38} for (Mn,Fe)Si made by the same research group with comparable Fe concentration. This puts the present system into the “highly disordered” region in refs. 34, 35, where a restoration of secondorder criticality is expected. For this region, the order parameter at T = 0 is predicted to show asymptotic critical behavior as m(Δp) ∝ (Δp)^{βQCP} as a function of pressure Δp = (p _{ QCP } − p), with the quantum critical exponent β _{ QCP } = 2/(d − 2 + λ) = 1.2 as shown in Table 1 of ref. 35 (third row of the fourth column, “Dirty (preasymptotic)”, with dimension d = 3 and the effective exponent λ = 2/3). The present results fit well to the relation σ (T → 0) ∝ (Δp)^{βQCP} with the orderparameter exponent β _{ QCP = }1.10 for p _{ c } = 23.0 kbar, and 0.80 for p _{ c } = 21.0 kbar. Although the present set of data cannot determine the value of beta more precisely due to uncertainty in the critical pressure p _{ c } at the QCP, these values are unquestionably different from the power β _{ QCP } = 0.5 (second column of Table 1^{35}) expected in calculations without including large disorder. To this extent, the present results are quantitatively consistent with the theoretical prediction. Further theoretical studies, however, may be helpful to discuss the possible effect of the Dzyaloshinskii–Moriya interaction and to elucidate any relationship with different theoretical approaches.^{39}
Strong sensitivity of firstorder behavior to disorder in pure MnSi was also found in acsusceptibility measurements, which showed a discontinuous T dependence of the susceptibility at T _{ C } for p* < p < p _{ c } for a very pure specimen with RRR = 243, while a continuous gradual change was observed for a less clean specimen with RRR = 40, as demonstrated in Figs. 5 and 7 in ref. 11 A MuSR study^{28} of a sample of MnSi with RRR = 40 reported firstorder quantum evolution but no phase separation at T → 0, in apparent disagreement with ref. 13 which found both first order evolution and phase separation at p* < p < p _{ c } in a cleaner crystal with RRR ~ 100. This difference may be related to a general tendency toward secondorder behavior in less clean systems.
The red filled circles in the phase diagram of Fig. 1a mark the critical temperature T _{ C } of (Mn_{0.85}Fe_{0.15})Si as determined from the peak position of 1/T _{ 1 }. It is quite interesting that the QCP of (Mn_{0.85}Fe_{0.15})Si at p ~ 21–23 kbar coincides with the extrapolation of the linear T _{ C }(p < p*) trend of MnSi to T = 0. Thus, the (Mn,Fe) substitution restored secondorder quantum criticality and even revealed the QCP in pure MnSi hidden by the firstorder thermal and quantum transitions for p > p*.
We note that phase separation of paramagnetic and magnetically ordered volumes is observed in many systems, including substitutiontuned (Sr,Ca)RuO_{3} ^{13} and RENiO_{3} (RE = rare earth), pressuretuned V_{2}O_{3},^{40} and highT _{c} cuprates with substitution and pressure tuning.^{41, 42} It may seem counterintuitive to imagine that greater disorder could help restore sharp features and secondorder criticality near a QCP, since disorder often “smears out” sharp features. On the other hand, percolation networks and dilutealloy spin glasses, which involve large amounts of disorder, exhibit secondorder critical behavior, such as that illustrated in Fig. 1d. It would then be highly interesting to determine whether the present observation of the role of disorder for an itinerantelectron system could be extended to the cases of quantum phase transitions in other metallic ferromagnets,^{43} Mott transitions systems, insulating magnets, and geometrically frustrated and/or low dimensional magnetic system.
Previous studies of quantum criticality in (Mn,Fe)Si have been performed mostly in ambient pressure with Fe composition as the tuning parameter.^{14, 44, 45} Near the disappearance of magnetic order, which occurs for Fe concentrations of approximately 0.16–0.19, a continuous reduction of the ordered moment size was noticed. This suggests a tendency toward secondorder criticality, consistent with the present results via pressure tuning. However, the present MuSR study provides some additional benefits beyond these earlier studies, in particular by involving only a fixed amount of disorder in a single sample, independently distinguishing the effects of pressure on moment size and volume fraction, and providing information on both the static order parameter and the dynamic critical behavior. Furthermore, the unexpected finding that the critical pressure for Fe 15% (Mn,Fe)Si is even larger than that of pure MnSi demonstrates that pressure and substitution tune the electronic structure not in a simple additive manner but in a more complicated way.
In conclusion, we demonstrated that the firstorder thermal and quantum phase transitions in pure MnSi near QCP are replaced by secondorder thermal and quantum transitions in (Mn_{0.85}Fe_{0.15})Si. The QCP in MnSi, hidden in the pure compound by a preceding firstorder quantum phase transition, is now revealed in (Mn,Fe)Si through the restorative effects of disorder. Up to now, most of the evidence for magnetic secondorder quantum criticality have been based on magnetization, transport, or neutron scattering experiments, which reflect volumeintegrated properties insensitive to phase separation. Together with the previous work^{13} in pure MnSi, the present work in (Mn,Fe)Si has demonstrated the importance of using a volumesensitive probe for elucidating quantum phase transitions. This work also demonstrates that for studying possible roles of disorder, quantum tuning with hydrostatic pressure and a fixed amount of disorder provides unambiguous information, in contrast to the uncertainty arising from varying degrees of disorder inherent in substitution tuning.
Methods
In positive MuSR (μ^{+}SR) measurements, spinpolarized positive muons are implanted in the specimen for condensed matter physics studies. In the case of measurements under applied pressure at PSI, a highmomentum (60–125 MeV/c) muon beam generated from pions decaying in flight must be used so that the muons can penetrate the pressure cell and reach the specimen. After losing its kinetic energy within 1 ns after implantation, the muon stops at an interstitial site in the specimen (or the wall of the pressure cell), and usually rests there with a mean lifetime of 2.2 μs until it decays and emits a positron. The angular distribution of positron emission is maximal along the muon spin direction at the time of decay. For the dc muon beam facilities at PSI and TRIUMF, beam collimation and logic circuits ensure that only one muon exists within the specimen at a given time. The time spectra of positron events F(t) and B(t), where t is the time after muon implantation, are recorded by two sets of counters, labeled forward (F) and backward (B), that are placed in front of and behind the sample with respect to the initial muon spin direction. After normalizing the solidangle factors between the two counters, the ratio [B(t) − F(t)]/[F(t) + B(t)] represents the time evolution of muon spin polarization AG(t), where A = 0.2–0.3 is the initial decay asymmetry and G(t) denotes the muon spin relaxation function. In the present paper, the time spectra AG(t) are displayed in Fig. 2. A discussion of relaxation functions in various systems can be found in ref. 33, while technical details of the measurements under applied pressure at PSI are described in ref. 32.
In MuSR, muons stopping in different environments contribute additively to the observed asymmetry AG(t). In the present study, out of total initial asymmetry of A ~ 0.27, the contributions from the specimen, pressure cell wall, and other backgrounds were approximately 0.12, 0.12, and 0.03, respectively, as described in the Supplementary Information (SI). This implies that about 40% of the total signal came from the specimen. Similarly, if there are two different phases in the specimen, the signals from different regions (phases) can be observed as different additive responses. In the present analyses, the observed signal from the specimen was decomposed into a signal from the magnetically ordered volumes with the temperaturedependent initial asymmetry A _{ 1 }(T) and a signal from the paramagnetic volume with A _{ 2 }(T), as shown in the SI. This allows a determination of the ordered volume fraction f _{mag} = A _{ 1 }/(A _{ 1 } + A _{ 2 } ), which is shown in Fig. 3a, c, e in the main text, for various temperatures T and pressures p.
The single crystal of (Mn,Fe)Si used in the present study was grown at Karlsruhe Institute of Technology by the vertical Bridgman technique from a stoichiometric mixture of Mn (4N), Fe (2N5+), and Si (5N) in an Al_{2}O_{3} crucible. A second crucible filled with pieces of Zr sponge was placed underneath the Bridgman crucible to getter gaseous impurities inside the working tube during crystal growth. Results for single crystals made by the same method as the present specimens were reported in ref. 38. The size of the present single crystal and the ratio of the signals from the specimen and the pressure cell wall are described in the SI.
Data availability
The data of the MuSR measurements discussed in this work were obtained using the GPD instrument at PSI. They can be accessed at the PSI web site http://musruser.psi.ch/cgibin/SearchDB.cgi, as Run # 706 – # 1175 of the year 2009.
References
 1.
Uchida, S. High Temperature Superconductivity: The Road to Higher Critical Temperature (Springer Verlag, 2015).
 2.
Keimer, B., Kivelson, S. A., Norman, M. R., Uchida, S. & Zaanen, J. From quantum matter to hightemperature superconductivity in copper oxides. Nature 518, 179–186 (2015).
 3.
Uemura, Y. J. Commonalities in phase and mode. Nat. Mater 8, 253–255 (2009).
 4.
Mathur, N. D. et al. Magnetically mediated superconductivity in heavy fermion compounds. Nature 394, 39–43 (1994).
 5.
Pfleiderer, C. Superconducting phases of felectron compounds. Rev. Mod. Phys. 81, 1551–1624 (2009).
 6.
Imada, M., Fujimori, A. & Tokura, Y. Metalinsulator transitions. Rev. Mod. Phys. 70, 1039–1263 (1998).
 7.
Moriya, T. Spin Flucutations in Itinerant Electron Magnetism (SpringerVerlag, 1985).
 8.
Belitz, D., Kirkpatrick, T. R. & Vojta, T. First order transitions and multicritical points in weak itinerant ferromagnets. Phys. Rev. Lett. 82, 4707–4710 (1999).
 9.
Belitz, D., Kirkpatrick, T. R. & Rollbühler, J. Tricritical behavior in itinerant quantum ferromagnets. Phys. Rev. Lett. 94, 247205 (2005).
 10.
Janoschek, M. et al. Fluctuationinduced firstorder phase transition in DzyaloshinskiiMoriya helimagnets. Phys. Rev. B 87, 134407 (2013).
 11.
Pfleiderer, C., McMullan, G. J., Julian, S. R. & Lonzarich, G. G. Magnetic quantum phase transition in MnSi under hydrostatic pressure. Phys. Rev. B 55, 8330–8338 (1997).
 12.
Pfleiderer, C. et al. Partial order in the nonFermiliquid phase of MnSi. Nature 427, 227–231 (2004).
 13.
Uemura, Y. J. et al. Phase separation and suppression of critical dynamics at quantum phase transitions of MnSi and (Sr_{1−x}Ca_{x})RuO_{3}. Nat. Phys. 3, 29–35 (2007).
 14.
Bauer, A. et al. Quantum phase transitions in singlecrystal Mn_{1−x}Fe_{x}Si and Mn_{1−x}Co_{x}Si: Crystal growth, magnetization, ac susceptibility, and specific heat. Phys. Rev. B 82, 064404 (2010).
 15.
Svanidze, E. Nonfermi liquid behavior close to a quantum critical point in a ferromagnetic state without local moments. Phys. Rev. X 5, 011026 (2015).
 16.
Ishikawa, Y., Noda, Y., Uemura, Y. J., Majkrzak, C. F. & Shirane, G. Paramagnetic Spin Fluctuations in the Weak Itinerant Ferromagnet MnSi. Phys. Rev. B 31, 5884–5893 (1985).
 17.
Hayano, R. S. et al. Observation of the T/(T − T_{c}) divergence of the μ^{+} spin relaxation rate in MnSi near T_{c}. Phys. Rev. Lett. 41, 1743–1746 (1978).
 18.
Muehlbauer, S. et al. Skyrmion lattice in a chiral magnet. Science 323, 915–919 (2009).
 19.
Yu, X. Z. Realspace observation of a twodimensional skyrmion crystal. Nature 465, 901–904 (2010).
 20.
Roessli, B., Böni, P., Fischer, W. E. & Endoh, Y. Chiral fluctuations in MnSi above the curie temperature. Phys. Rev. Lett. 88, 237204 (2002).
 21.
Grigoriev, S. V. et al. Critical fluctuations in MnSi near T_{C}: A polarized neutron scattering study. Phys. Rev. B 72, 134420 (2005).
 22.
Pappas, C. et al. Magnetic fluctuations and correlations in MnSi: Evidence for a chiral skyrmion spin liquid phase. Phys. Rev. B 83, 224405 (2011).
 23.
Stishov, S. M. & Petrova, A. E. Itinerant helimagnet MnSi. Phys. Uspekhi 54, 1117–1130 (2011).
 24.
Takigawa, M. et al. Positive muon spin rotation and relaxation in the helically ordered state of MnSi. J. Phys. Soc. Jpn. 49, 1760–1767 (1980).
 25.
Yaouanc, A. et al. Testing the selfconsistent renormalization theory for the description of the spinfluctuation modes of MnSi at ambient pressure. J. Phys. Condens. Matter 17, 129–135 (2005).
 26.
GatMaruleanu, I. M. et al. Field dependence of muon spin relaxation rate in MnSi. Phys. Rev. Lett. 90, 157201 (2003).
 27.
Yu, W. et al. Phase inhomogeneity of the itinerant ferromagnet MnSi at high pressures. Phys. Rev. Lett. 92, 086403 (2004).
 28.
Andreica, D., Dalmas de Réotier, P., Yaouanc, A., Amato, A. & Lapertot, G. Absence of magnetic phase separation in MnSi under pressure. Phys. Rev. B81 060412(R) (2010).
 29.
Fåk, B., Sadykov, R.A., Flouquet, J., Lapertot, G. Pressure dependence of the magnetic structure of the itinerant electron magnet MnSi. J. Phys. Condens. Matter 17, 1635–1644 (2005).
 30.
Pfleiderer, C., Reznik, D., Pintschovius, L. & Haug, J. Magnetic Field and Pressure Dependence of Small Angle Neutron Scattering in MnSi. Phys. Rev. Lett. 99, 156406 (2007).
 31.
Manyala, N. et al. Large anomalous Hall effect in a siliconbased magnetic semiconductor. Nat. Mater. 3, 255–262 (2004).
 32.
Khasanov, R. et al. High pressure research using muons at the Paul Scherrer Institute. High Press Res. 36, 140–166 (2016).
 33.
Uemura, Y. J. µSR relaxation functions in magnetic materials. In Muon Science: Muons in Physics, Chemistry and Materials Proceedings of the Fifty First Scottish Universities Summer School in Physics, (eds Lee, S. L., Kilcoyne, S. H. & Cywinski, R.) 85–114 (Inst. of Physics Publishing, 1999).
 34.
Sang, Y., Belitz, D. & Kirkpatrick, T. R. Disorder Dependence of the Ferromagnetic Quantum Phase Transition. Phys. Rev. Lett. 113, 207201 (2014).
 35.
Kirkpatrick, T. R. & Belitz, D. Exponent relations at quantum phase transitions with applications to metallic quantum ferromagnets. Phys. Rev. B 91, 214407 (2015).
 36.
Kirkpatrick, T. R. & Belitz, D. Third law of thermodynamics and the shape of the phase diagram for systems with a firstorder quantum phase transition. Phys. Rev. Lett. 115, 020402 (2015).
 37.
Kirkpatrick, T. R. & Belitz, D. Stable phase separation and heterogeneity away from coexistence curve. Phys. Rev. B 93, 144203 (2016).
 38.
Chapman, B. J., Grossnickle, M. G., Wolf, T. & Lee, M. Large enhancement of emergent magnetic fields in MnSi with impurities and pressure. Phys. Rev. B 88, 214406 (2013).
 39.
Krüger, F., Karahasanovic, U. & Green, A. G. Quantum orderbydisorder near criticality and the secret of partial order in MnSi. Phys. Rev. Lett. 108, 067003 (2012).
 40.
Frandsen, B. A. et al. Volumewise destruction of the antiferromagnetic Mott insulating state through quantum tuning. Nat. Commun. 7, 12519 (2016).
 41.
Kojima, K. M. et al. Superfluid density and volume fraction of static magnetism in stripestabilized La_{1.85−y}Eu_{y}Sr_{0.15}CuO_{4}. Physica B36, 316–320 (2003).
 42.
Guguchia, Z. et al. Tuning the static spinstripe phase and superconductivity in La_{2−x}Ba_{x}CuO_{4} (x = 1/8) by hydrostatic pressure. New J. Phys. 15, 093005 (2013).
 43.
Brando, M., Belitz, D., Grosche, F. M. & Kirkpatrick, T. R. Metallic quantum ferromagnets. Rev. Mod. Phys. 88, 025006 (2016).
 44.
Franz, C. et al. Realspace and reciprocalspace berry phases in the Hall effect of Mn_{1−x}Fe_{x}Si. Phys. Rev. Lett. 112, 186601 (2014).
 45.
Glushkov, V. V. et al. Scrutinizing Hall effect in Mn_{1−x}Fe_{x}Si: Fermi surface evolution and hidden quantum criticality. Phys. Rev. Lett. 115, 256601 (2015).
Acknowledgements
The authors would like to thank Dietrich Belitz, Andy Millis and Christian Pfleiderer for useful discussions, and Benjamin Frandsen for editing English of the manuscript. Work at Columbia was supported by the US National Science Foundation grants DMR1105961, DMR1436095 (DMREF grant), DMR1610633, OISE0968226 (PIRE), the Japan Atomic Energy Agency Reimei project during 2011–17, the Friends of University of Tokyo Inc. D.R. at the University of Colorado Boulder was supported by the US DOE, Office of Basic Energy Sciences, Materials Sciences and Engineering Division under Contract No. DESC0006939, and M.L. was supported by the US DOE, Basic Energy Sciences, Materials Sciences and Engineering Division under Award Number DESC0006888. The MuSR measurements were performed at the Swiss Muon Source (SμS), PSI, Villigen, Switzerland.
Author information
Affiliations
Contributions
Y.J.U. and D.R. conceived the experiment, T.W. prepared the single crystal specimen, T.G. designed the pressure cell, T.G., C.J.A., Y.J.U., A.H., D.R., A.M., R.K., and E.M. performed MuSR measurements at PSI, M.L. performed resistivity measurements on relevant crystals, and T.G. and Y.J.U. performed data analysis and drafted the manuscript, which was then revised and agreed upon by all the authors.
Corresponding author
Ethics declarations
Competing Interests
The authors declare that they have no competing financial interests.
Additional information
Publisher's note: Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Electronic supplementary material
Rights and permissions
Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/.
About this article
Cite this article
Goko, T., Arguello, C.J., Hamann, A. et al. Restoration of quantum critical behavior by disorder in pressuretuned (Mn,Fe)Si. npj Quant Mater 2, 44 (2017). https://doi.org/10.1038/s4153501700490
Received:
Revised:
Accepted:
Published:
Further reading

Disorderinduced critical exponents near a ferromagnetic quantum critical point in Mn1−xCrxSi
Physical Review B (2020)

Ferromagnetic Quantum Critical Point in Noncentrosymmetric Systems
Physical Review Letters (2020)

The emergent field of high entropy oxides: Design, prospects, challenges, and opportunities for tailoring material properties
APL Materials (2020)

Quantum Critical Point in the Itinerant Ferromagnet Ni1−xRhx
Physical Review Letters (2020)

Spin dynamics and a nearly continuous magnetic phase transition in an entropystabilized oxide antiferromagnet
Physical Review Materials (2020)